LMucko/crystallography-open-database huggingface dataset:
Electron density study of a new non-linear optical material: <small>L</small>-arginine phosphate monohydrate (LAP). Comparison between <i>X</i>–<i>X</i> and <i>X</i>–(<i>X</i> + <i>N</i>) refinements
Espinosa, E.; Lecomte, C.; Molins, E.; Veintemillas, S.; Cousson, A.; Paulus, W.; Acta Crystallographica Section B 52 (1996) 519–534; doi:10.1107/S0108768195015205

data_2101536
_publ_section_title
;
 Electron density study of a new non-linear optical material:
 <small>L</small>-arginine phosphate monohydrate (LAP). Comparison
 between <i>X</i>--<i>X</i> and <i>X</i>--(<i>X</i> + <i>N</i>)
 refinements
;
_journal_issue                   3
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              519
_journal_page_last               534
_journal_paper_doi               10.1107/S0108768195015205
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'C6 H19 N4 O7 P'
_chemical_formula_weight         290.22
_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_Hall           'P 2yb'
_space_group_name_H-M_alt        'P 1 21 1'
_cell_angle_alpha                90.0
_cell_angle_beta                 98.00(10)
_cell_angle_gamma                90.0
_cell_formula_units_Z            2
_cell_length_a                   7.333(6)
_cell_length_b                   7.93(2)
_cell_length_c                   10.81(2)
_cell_measurement_reflns_used    16
_cell_measurement_temperature    130(5)
_cell_measurement_theta_max      16.2
_cell_measurement_theta_min      10.6
_cell_volume                     622.5
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     0.8302(2)
_exptl_absorpt_coefficient_mu    0.22
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.54
_exptl_crystal_description       prismatic
_exptl_crystal_size_max          3.5
_exptl_crystal_size_mid          3.0
_exptl_crystal_size_min          2.5
_cod_data_source_file            pa0310.cif
_cod_depositor_comments
;
 Added _atom_site_type_symbol label and values.

 Antanas Vaitkus
 2013-04-09
;
_cod_original_formula_sum        'C6 H19 N4 O7 P1'
_cod_database_code               2101536
Electron density study of a new non-linear optical material: <small>L</small>-arginine phosphate monohydrate (LAP). Comparison between <i>X</i>–<i>X</i> and <i>X</i>–(<i>X</i> + <i>N</i>) refinements
Espinosa, E.; Lecomte, C.; Molins, E.; Veintemillas, S.; Cousson, A.; Paulus, W.; Acta Crystallographica Section B 52 (1996) 519–534; doi:10.1107/S0108768195015205

data_2101537
_publ_section_title
;
 Electron density study of a new non-linear optical material:
 <small>L</small>-arginine phosphate monohydrate (LAP). Comparison
 between <i>X</i>--<i>X</i> and <i>X</i>--(<i>X</i> + <i>N</i>)
 refinements
;
_journal_issue                   3
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              519
_journal_page_last               534
_journal_paper_doi               10.1107/S0108768195015205
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'C6 H19 N4 O7 P'
_chemical_formula_weight         290.22
_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_Hall           'P 2yb'
_space_group_name_H-M_alt        'P 1 21 1'
_cell_angle_alpha                90.0
_cell_angle_beta                 98.05(2)
_cell_angle_gamma                90.0
_cell_formula_units_Z            2
_cell_length_a                   7.3190(10)
_cell_length_b                   7.912(2)
_cell_length_c                   10.779(3)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    130(3)
_cell_measurement_theta_max      28
_cell_measurement_theta_min      13
_cell_volume                     618.0
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    0.24
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.54
_exptl_crystal_description       prismatic
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.26
_exptl_crystal_size_min          0.22
_cod_data_source_file            pa0310.cif
_cod_depositor_comments
;
 Added _atom_site_type_symbol label and values.

 Antanas Vaitkus
 2013-04-09
;
_cod_original_formula_sum        'C6 H19 N4 O7 P1'
_cod_database_code               2101537
Electron density study of a new non-linear optical material: <small>L</small>-arginine phosphate monohydrate (LAP). Comparison between <i>X</i>–<i>X</i> and <i>X</i>–(<i>X</i> + <i>N</i>) refinements
Espinosa, E.; Lecomte, C.; Molins, E.; Veintemillas, S.; Cousson, A.; Paulus, W.; Acta Crystallographica Section B 52 (1996) 519–534; doi:10.1107/S0108768195015205

data_2101538
_publ_section_title
;
 Electron density study of a new non-linear optical material:
 <small>L</small>-arginine phosphate monohydrate (LAP). Comparison
 between <i>X</i>--<i>X</i> and <i>X</i>--(<i>X</i> + <i>N</i>)
 refinements
;
_journal_issue                   3
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              519
_journal_page_last               534
_journal_paper_doi               10.1107/S0108768195015205
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'C6 H19 N4 O7 P'
_chemical_formula_weight         290.22
_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_Hall           'P 2yb'
_space_group_name_H-M_alt        'P 1 21 1'
_cell_angle_alpha                90.0
_cell_angle_beta                 98.05(2)
_cell_angle_gamma                90.0
_cell_formula_units_Z            2
_cell_length_a                   7.3190(10)
_cell_length_b                   7.912(2)
_cell_length_c                   10.779(3)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    130(3)
_cell_measurement_theta_max      28
_cell_measurement_theta_min      13
_cell_volume                     618.0
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    0.24
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.54
_exptl_crystal_description       prismatic
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.26
_exptl_crystal_size_min          0.22
_cod_data_source_file            pa0310.cif
_cod_depositor_comments
;
 Added _atom_site_type_symbol label and values.

 Antanas Vaitkus
 2013-04-09
;
_cod_original_formula_sum        'C6 H19 N4 O7 P1'
_cod_database_code               2101538
Distance limits of OH···<i>Y</i> hydrogen bonds (<i>Y</i> = Cl, Br, I) in solid hydroxides, structure refinement of laurionite-type Ba(OD)I, Sr(OD)I and Sr(OH)I by neutron and synchrotron X-ray powder diffraction
Peter, S.; Cockcroft, J. K.; Roisnel, T.; Lutz, H. D.; Acta Crystallographica Section B 52 (1996) 423–427; doi:10.1107/S0108768195013449

data_2101539
_publ_section_title
;
 Distance limits of OH&#x00B7;&#x00B7;&#x00B7;<i>Y</i> hydrogen bonds
 (<i>Y</i> = Cl, Br, I) in solid hydroxides, structure refinement of
 laurionite-type Ba(OD)I, Sr(OD)I and Sr(OH)I by neutron and
 synchrotron X-ray powder diffraction
;
_journal_issue                   3
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              423
_journal_page_last               427
_journal_paper_doi               10.1107/S0108768195013449
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'H I O Sr'
_chemical_formula_weight         231.532
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   7.72940(10)
_cell_length_b                   4.24697(7)
_cell_length_c                   10.73740(10)
_cell_volume                     352.472(8)
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.85
_exptl_crystal_density_diffrn    4.362
_cod_data_source_file            se0177.cif
_cod_data_source_block           se0177a
_cod_depositor_comments
;
 Marking attached hydrogen atoms.

 Antanas Vaitkus,
 2017-03-27
;
_cod_original_cell_volume        352.470(10)
_cod_database_code               2101539
Crystal packing calculations and Rietveld refinement in elucidating the crystal structures of two modifications of 4-amidinoindanone guanylhydrazone
Karfunkel, H. R.; Wu, Z. J.; Burkhard, A.; Rihs, G.; Sinnreich, D.; Buerger, H. M.; Stanek, J.; Acta Crystallographica Section B 52 (1996) 555–561; doi:10.1107/S0108768195017174

data_2101542
_publ_section_title
;
 Crystal packing calculations and Rietveld refinement in elucidating
 the crystal structures of two modifications of 4-amidinoindanone
 guanylhydrazone
;
_journal_issue                   3
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              555
_journal_page_last               561
_journal_paper_doi               10.1107/S0108768195017174
_journal_volume                  52
_journal_year                    1996
_chemical_formula_moiety         'C11 H14 N6'
_chemical_formula_sum            'C11 H14 N6'
_chemical_formula_weight         230.27
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                71.078
_cell_angle_beta                 82.838
_cell_angle_gamma                78.941
_cell_formula_units_Z            2
_cell_length_a                   10.717
_cell_length_b                   7.762
_cell_length_c                   7.418
_cell_volume                     571.585
_diffrn_measurement_device       Guinier
_exptl_crystal_description       powder
_cod_data_source_file            sh0073.cif
_cod_data_source_block           sh0073a
_cod_original_cell_volume        571.59
_cod_database_code               2101542
Structure of the polytypic β-form of P~3~N~3~(OCH~2~CF~2~CF~2~CH~2~O)F~4~
Wang, Z.; Willett, R. D.; Elias, A. J.; Kirchmeier, R. L.; Shreeve, J. M.; Acta Crystallographica Section B 52 (1996) 643–650; doi:10.1107/S0108768195016089

data_2101552
_publ_section_title
;
 Structure of the polytypic \b-form of
 P~3~N~3~(OCH~2~CF~2~CF~2~CH~2~O)F~4~
;
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              643
_journal_page_last               650
_journal_paper_doi               10.1107/S0108768195016089
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'C4 H4 F8 N3 O2 P3'
_chemical_formula_weight         371.0
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                110.22(3)
_cell_angle_beta                 90.02(3)
_cell_angle_gamma                97.10(3)
_cell_formula_units_Z            12
_cell_length_a                   12.392(2)
_cell_length_b                   16.569(3)
_cell_length_c                   19.257(4)
_cell_volume                     3677.8(14)
_diffrn_radiation_type           Cu
_diffrn_radiation_wavelength     1.54184
_exptl_absorpt_coefficient_mu    5.584
_exptl_crystal_density_diffrn    2.010
_exptl_crystal_F_000             2184
_cod_data_source_file            cr0501.cif
_cod_data_source_block           cr0501a
_cod_original_cell_volume        3677.9(12)
_cod_database_code               2101552
Sodalite, Na~4~Si~3~Al~3~O~12~Cl: structure and ionic mobility at high temperatures by neutron diffraction
McMullan, R. K.; Ghose, S.; Haga, N.; Schomaker, V.; Acta Crystallographica Section B 52 (1996) 616–627; doi:10.1107/S0108768196004132

data_2101556
_publ_section_title
;
 Sodalite, Na~4~Si~3~Al~3~O~12~Cl: structure and ionic mobility at high
 temperatures by neutron diffraction
;
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              616
_journal_page_last               627
_journal_paper_doi               10.1107/S0108768196004132
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'Al3 Cl Na4 O12 Si3'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'P -4n 2 3'
_symmetry_space_group_name_H-M   'P -4 3 n'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            2
_cell_length_a                   8.8820(10)
_cell_length_b                   8.8820(10)
_cell_length_c                   8.8820(10)
_cell_volume                     700.70(14)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.05560(10)
_exptl_crystal_density_diffrn    2.297
_cod_data_source_file            cr0505.cif
_cod_data_source_block           cr0505a
_cod_original_cell_volume        700.7(2)
_cod_original_formula_sum        'Al3 Cl1 Na4 O12 Si3'
_cod_database_code               2101556
Experimental and theoretical morphologies of diuron, <i>N</i>'-(3,4-dichlorophenyl)-<i>N</i>,<i>N</i>-dimethylurea
Pfefer, G.; Boistelle, R.; Acta Crystallographica, Section B: Structural Science 52 (1996) 662–667; doi:10.1107/S010876819600047X

data_2101557
_publ_section_title
;
 Experimental and theoretical morphologies of diuron,
 <i>N</i>'-(3,4-dichlorophenyl)-<i>N</i>,<i>N</i>-dimethylurea
;
_journal_coden_ASTM              ASBSDK
_journal_coeditor_code           DU0403
_journal_issue                   4
_journal_name_full
;
 Acta Crystallographica, Section B: Structural Science
;
_journal_page_first              662
_journal_page_last               667
_journal_paper_doi               10.1107/S010876819600047X
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'C9 H10 Cl2 N2 O'
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yab'
_space_group_name_H-M_alt        'P 1 21/a 1'
_cell_angle_alpha                90.0
_cell_angle_beta                 101.32
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   9.191
_cell_length_b                   14.632
_cell_length_c                   7.738
_diffrn_radiation_type           Mo
_diffrn_radiation_wavelength     0.71073
_cod_data_source_file            du0403.cif
_cod_depositor_comments
;
 Adding the _atom_site_type_symbol data item and the ATOM_TYPE loop.

 Antanas Vaitkus,
 2018-08-12

 Updating space group information.

 Antanas Vaitkus,
 2018-08-12
;
_cod_original_formula_sum        'C9 H10 Cl2 N2 O1'
_cod_database_code               2101557
Structure of Ce~2~Pt~6~Ga~15~: interplanar disorder from the Ce~2~Ga~3~ layers
Kwei, G. H.; Lawson, A. C.; Larson, A. C.; Morosin, B.; Larson, E. M.; Canfield, P. C.; Acta Crystallographica Section B 52 (1996) 580–585; doi:10.1107/S0108768196000481

data_2101568
_publ_section_title
;
 Structure of Ce~2~Pt~6~Ga~15~: interplanar disorder from the
 Ce~2~Ga~3~ layers
;
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              580
_journal_page_last               585
_journal_paper_doi               10.1107/S0108768196000481
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'Ce2 Ga15 Pt6'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            1.5
_cell_length_a                   4.3267(2)
_cell_length_b                   4.3267(2)
_cell_length_c                   16.5369(8)
_cell_volume                     268.10(2)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           'pulsed neutron'
_cod_data_source_file            vs0127.cif
_cod_data_source_block           vs0127a
_cod_original_cell_volume        268.11(3)
_cod_database_code               2101568
Structure of Ce~2~Pt~6~Ga~15~: interplanar disorder from the Ce~2~Ga~3~ layers
Kwei, G. H.; Lawson, A. C.; Larson, A. C.; Morosin, B.; Larson, E. M.; Canfield, P. C.; Acta Crystallographica Section B 52 (1996) 580–585; doi:10.1107/S0108768196000481

data_2101569
_publ_section_title
;
 Structure of Ce~2~Pt~6~Ga~15~: interplanar disorder from the
 Ce~2~Ga~3~ layers
;
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              580
_journal_page_last               585
_journal_paper_doi               10.1107/S0108768196000481
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'Ce2 Ga15 Pt6'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            1.5
_cell_length_a                   4.335(10)
_cell_length_b                   4.335(10)
_cell_length_c                   16.564(7)
_cell_volume                     269.6(9)
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_cod_data_source_file            vs0127.cif
_cod_data_source_block           vs0127b
_cod_original_cell_volume        269.7(2)
_cod_database_code               2101569
Structure of Ce~2~Pt~6~Ga~15~: interplanar disorder from the Ce~2~Ga~3~ layers
Kwei, G. H.; Lawson, A. C.; Larson, A. C.; Morosin, B.; Larson, E. M.; Canfield, P. C.; Acta Crystallographica Section B 52 (1996) 580–585; doi:10.1107/S0108768196000481

data_2101570
_publ_section_title
;
 Structure of Ce~2~Pt~6~Ga~15~: interplanar disorder from the
 Ce~2~Ga~3~ layers
;
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              580
_journal_page_last               585
_journal_paper_doi               10.1107/S0108768196000481
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'Ce2 Ga15 Pt6'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            1.5
_cell_length_a                   4.3259(5)
_cell_length_b                   4.3259(5)
_cell_length_c                   16.522(3)
_cell_volume                     267.76(7)
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           'pulsed neutron'
_cod_data_source_file            vs0127.cif
_cod_data_source_block           vs0127c
_cod_original_cell_volume        267.760(10)
_cod_database_code               2101570
Prediction of ferroelectricity in recent Inorganic Crystal Structure Database entries under space group <i>Pba</i>2
Abrahams, S. C.; Mirsky, K.; Nielson, R. M.; Acta Crystallographica Section B 52 (1996) 806–809; doi:10.1107/S0108768196004582

data_2101572
_publ_section_title
;
 Prediction of ferroelectricity in recent Inorganic Crystal Structure
 Database entries under space group <i>Pba</i>2
;
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              806
_journal_page_last               809
_journal_paper_doi               10.1107/S0108768196004582
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'C H8 F6 N4 Zr'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'P 2 -2ab'
_symmetry_space_group_name_H-M   'P b a 2'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_length_a                   10.089(2)
_cell_length_b                   18.349(3)
_cell_length_c                   7.5600(10)
_cell_volume                     1399.5(4)
_diffrn_radiation_type           Mo
_diffrn_radiation_wavelength     0.71073
_cod_data_source_file            an0526.cif
_cod_data_source_block           an0526a
_cod_original_formula_sum        'C1 H8 F6 N4 Zr1'
_cod_database_code               2101572
Prediction of ferroelectricity in recent Inorganic Crystal Structure Database entries under space group <i>Pba</i>2
Abrahams, S. C.; Mirsky, K.; Nielson, R. M.; Acta Crystallographica Section B 52 (1996) 806–809; doi:10.1107/S0108768196004582

data_2101573
_publ_section_title
;
 Prediction of ferroelectricity in recent Inorganic Crystal Structure
 Database entries under space group <i>Pba</i>2
;
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              806
_journal_page_last               809
_journal_paper_doi               10.1107/S0108768196004582
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'Ba0.6 Bi K0.4 O2.3'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'P 2 -2ab'
_symmetry_space_group_name_H-M   'P b a 2'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_length_a                   6.127
_cell_length_b                   12.016
_cell_length_c                   4.378
_cell_volume                     322.317
_diffrn_radiation_type           Mo
_diffrn_radiation_wavelength     0.71073
_cod_data_source_file            an0526.cif
_cod_data_source_block           an0526b
_cod_original_formula_sum        'Ba0.6 Bi1 K0.4 O2.3'
_cod_database_code               2101573
Prediction of ferroelectricity in recent Inorganic Crystal Structure Database entries under space group <i>Pba</i>2
Abrahams, S. C.; Mirsky, K.; Nielson, R. M.; Acta Crystallographica Section B 52 (1996) 806–809; doi:10.1107/S0108768196004582

data_2101574
_publ_section_title
;
 Prediction of ferroelectricity in recent Inorganic Crystal Structure
 Database entries under space group <i>Pba</i>2
;
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              806
_journal_page_last               809
_journal_paper_doi               10.1107/S0108768196004582
_journal_volume                  52
_journal_year                    1996
_chemical_formula_sum            'Cl10 Mo N O P2'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'P 2 -2ab'
_symmetry_space_group_name_H-M   'P b a 2'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_length_a                   15.984(2)
_cell_length_b                   11.412(2)
_cell_length_c                   4.1510(10)
_cell_volume                     757.2(2)
_diffrn_radiation_type           Mo
_diffrn_radiation_wavelength     0.71073
_cod_data_source_file            an0526.cif
_cod_data_source_block           an0526c
_cod_original_formula_sum        'Cl10 Mo1 N1 O1 P2'
_cod_database_code               2101574